biosynthesis of biocompatible cadmium telluride quantum ... cadmium telluride (cdte) quantum dots,...
Post on 25-Jun-2020
Embed Size (px)
Nano Res (2010) 3: 481–489
Biosynthesis of Biocompatible Cadmium Telluride Quantum Dots Using Yeast Cells
Haifeng Bao, Na Hao, Yunxia Yang, and Dongyuan Zhao ( ) Department of Chemical Engineering, Monash University, Clayton, VIC3800, Australia Received: 14 April 2010 / Revised: 9 May 2010 / Accepted: 11 May 2010 © The Author(s) 2010. This article is published with open access at Springerlink.com
ABSTRACT We demonstrate a simple and efficient biosynthesis method to prepare easily harvested biocompatible cadmium telluride (CdTe) quantum dots (QDs) with tunable fluorescence emission using yeast cells. Ultraviolet–visible (UV–vis) spectroscopy, photoluminescence (PL) spectroscopy, X-ray diffraction (XRD), and transmission electron microscopy (TEM) confirm that the CdTe QDs are formed via an extracellular growth and subsequent endocytosis pathway and have size-tunable optical properties with fluorescence emission from 490 to 560 nm and a cubic zinc blende structure with good crystallinity. In particular, the CdTe QDs with uniform size (2–3.6 nm) are protein-capped, which makes them highly soluble in water, and in situ bio-imaging in yeast cells indicates that the biosynthesized QDs have good biocompatibility. This work provides an economic and environmentally friendly approach to synthesize highly fluorescent biocompatible CdTe QDs for bio-imaging and bio-labeling applications. KEYWORDS Cadmium telluride (CdTe) quantum dots, biosynthesis, biocompatible, in situ bio-imaging
Semiconductor nanocrystal quantum dots (QDs) exhibit unique size-dependent electronic and optical properties due to the quantum confinement effect [1, 2]. To date, many kinds of QDs with different size, shape, and composition [3–5] have been extensively investigated for not only their theoretical fundamentals but also their practical applications, including in solar cells , optoelectronic transistor components , and fluorescent biological labels [8, 9]. Among various QDs, cadmium telluride (CdTe) QDs have been widely used in industrial and biomedical applications [7, 10–12] because of their tunable photoluminescence within
the visible range when excited by a single excitation wavelength. For instance, CdTe QDs are believed to be promising probes in the bio-imaging of living cells  because of their many advantages such as higher photostability, more controllable and narrower emission bands, and higher quantum yield in com- parison with conventional fluorescent dyes. To date, two successful routes for the synthesis of highly fluorescent CdTe QDs have been developed, namely the organometallic method [3, 14, 15] and water-based synthesis [16–19] with thiols as capping ligands. However, these reactions need to be performed at high temperature. Moreover, the resulting QDs need to be attached with proteins or capped with layers of
Nano Res (2010) 3: 481–489 DOI 10.1007/s12274-010-0008-6 Research Article
Address correspondence to firstname.lastname@example.org
Nano Res (2010) 3: 481–489
low toxicity in order to decrease their toxicity in bio-imaging and bio-labeling applications [5, 10]. The development of a cheap, effective, and reproducible method to prepare CdTe QDs with controlled structures and properties on a large scale remains a great challenge.
More recently, the biosynthesis of QDs has been developed and attracted significant attention. This involves the use of biological organisms to prepare QDs with controlled size, shape, chemical composition, and functionality . For example, several micro- organisms including Fusarium oxysporum  and Schizosaccharomyces pombe  have been employed to synthesize CdS QDs, whilst Torulopsis species  have been used to prepare PbS QDs, and sulfate reducing bacteria and Rhodobacter sphaeroides to synthesize ZnS QDs . Sweeney et al. reported that CdS QDs can be formed intracellularly in E. coli cells incubated with cadmium chloride and sodium sulfide . All these environmentally friendly approaches are achieved at ambient temperatures. However, complicated procedures are required to isolate the intracellularly grown QDs and the photoluminescence of these biosynthesized QDs has been seldom reported [26–28]. Therefore, it is of great importance to develop a simple and cheap biosynthesis approach which can prepare highly fluorescent QDs with uniform size and extend their biological applications, especially for CdTe QDs—one of the most popular nanocrystals.
In this paper, we demonstrate a simple and efficient biosynthesis of highly fluorescent CdTe QDs with uniform size (2.0–3.6 nm) by incubating a type of widely used and easily cultured microorganism—yeast cells (Saccharomyces cerevisiae)—with cheap inorganic Cd and Te salt precursors, which has a high yield of nearly 90%. The extracellularly bio-grown CdTe QDs can be easily harvested and display tunable size- dependent emission from 490 to 560 nm with a relatively high photoluminescence (PL) quantum yield of ~33% due to their high crystallinity. Furthermore, the CdTe QDs are naturally capped with proteins in the biosystem, and show excellent water solubility, great stability, and biocompatibility. Our work can not only provide an economic and environmentally friendly route to prepare highly fluorescent biocompatible CdTe
QDs on a gram scale, but also extend bio-imaging and bio-labeling applications of biosynthesized QDs.
Cadmium chloride hemipentahydrate (CdCl2·2.5H2O), sodium citrate tribasic dihydrate (C6H5O7Na3·2H2O), sodium tellurite (Na2TeO3) (100 mesh, 99%), mercap- tosuccinic acid (MSA), sodium borohydride (NaBH4, 99.995%), sodium nitrate (NaNO3), dipotassium hydrogenphosphate (K2HPO4), potassium chloride (KCl), magnesium sulfate hepta-hydrate (MgSO4·7H2O), Rhodamine 6G, and ethanol (anhydrous, ≥ 99.95%) were purchased from Sigma–Aldrich Corporation. All these chemicals were used without further purification. The water was deionized through a Nex Power 1000 water purification system (Human Corporation).
The yeast cells were grown with aeration at 35 °C in a modified Czapek’s medium. In a typical procedure, 450 g of sucrose, 15 g of NaNO3, 5.0 g of K2HPO4, 2.5 g of KCl, 2.5 g of MgSO4·7H2O, and 30.0 g of sodium citrate tribasic dihydrate were dissolved in 5 L of deionized water under stirring and placed in a 5000 mL conical flask and incubated with yeast cells for 2 days at 35 °C. When the absorbance of the cell culture reached 0.6 at 600 nm (A600), the resulting yeast solution was added with 400 mL of cadmium chloride (CdCl2) (0.04 mol/L), 100 mL of Na2TeO3 (0.04 mol/L), 7.5 g of MSA, and 5.0 g of NaBH4, followed by incubation at 35 °C in a water bath with continuous stirring (500 r/min). The biosynthesized CdTe QDs were centrifuged at 5000 r/min for 15 min to remove the yeast cells, and dialyzed three times at room temperature (25 °C) by using a dialysis membrane (MWCO-14 000, USA) to remove the residual chemicals. Finally, 1.15 g of as-biosyn-thesized CdTe QD products was obtained with a yield of nearly 90%, calculated from the amount of Na2TeO3. The capped proteins were obtained by treating the as-biosynthesized CdTe QDs with HCl to dissolve the CdTe for the high-performance liquid chromatography (HPLC) measurements.
Nano Res (2010) 3: 481–489
X-ray powder diffraction (XRD) patterns were recorded using a Bruker D8 X-ray diffractometer (Germany) with Ni-filtered Cu Kα radiation (40 kV, 40 mA). Transmission electron microscopy (TEM) and high- resolution TEM (HRTEM) images were taken with a JEM-2100F (UHR) (JEOL, Japan) electron microscope operating at 200 kV. TEM samples were prepared by dropping suspensions on copper grids and dried at room temperature (25 °C) for 24 h. After incubation for different durations, the crude solution was centrifuged at 5000 r/min for 10 min to precipitate the yeast. The supernatant was collected for the measurement of the ultraviolet–visible (UV–vis) and PL spectra. The optical characterizations were performed at room temperature (25 °C). UV–vis absorption spectra were recorded on a Cary 500 UV/Vis/near-infrared (IR) Varian spectrophotometer (USA). PL spectra were obtained with a PerkinElmer LS 55 luminescence spectrometer (USA) with an excitation wavelength of 400 nm. The PL quantum yields of the biosynthesized CdTe QDs were calculated by comparison with a solution of Rhodamine 6G in anhydrous ethanol according to the procedure reported previously in Ref. . Laser scanning confocal microscopy (LSCM) measurements were carried out on Olympus FV1000 instrument with an Ar/Kr laser. The yeast cells were separated by centrifugation at 1000 r/min for the LSCM experiments. Fourier transform infrared (FT–IR) spectra were obtained with a PerkinElmer Spectrum 100 spectro- meter (USA) using KBr pellets. High-performance liquid chromatography (HPLC) was performed at 25 °C on a Waters 650E Advanced Protein Purification system (USA), with a Shim–Pack Diol-150 HPLC column (Shimadzu, Kyoto, Japan) equilibrated with 0.05 mol/L Na2SO4 at a flow rate of 1.0 mL/min and a gradient control monitoring the separation at 280 nm and with a Waters 486 tunable wavelength detector. The following molecular mass markers were used: Bovine serum albumin (BSA, 66.2 kD), alpha-chymotrypsin (25.0 kD), and lysozyme (14.4 kD). The relationship between the retention time (tR) and the molecular mass (M) can be expressed by a simple equa